of CuFe02 Single Crystals
P. DORDOR, J. P. CHAMINADE, A. WICHAINCHAI.* E. MARQUESTAUT, J. P. DOUMERC, M. POUCHARD, AND P. HAGENMULLER Lahowtoire de Chimie ELI Solidr du CNRS, Universitc; de Bordecrux I, 3.51, course de 10 LihPrution, 33405 Talencc Cedes, France AND
Luhoratoire de Chimie du Solide MinPral, FacultP des Sciences, Universite Cadi-Ayyad, Marrakech, Maroc Received
Delafossite-type CuFeO, single crystals have been prepared by a flux method: crystals obtained in a Cu crucible with LiBOz as flux are n-type whereas those prepared in a Pt crucible with a CuzO flux are p-type. Electrical measurements have revealed that n-type crystals exhibit weak anisotropic conductivities with large activation energies and small mobilities (r.t. values perpendicular and parallel to the c-axis: pL = 5 x 10ms and F, = lO~‘cm~’ V ’ set-I). p-type crystals, less anisotropic, are characterized by low activation energies and higher mobilities (pL_ = 34 and EL, = 8.9 cmz V’ set I). A twoconduction-band model is proposed to account for the difference observed between the energy gap value deduced from photoelectrochemical measurements and the activation energy of the electrical conductivity in the intrinsic domain. G 1988 Academic Pre\r. Inc.
Introduction Many studies have been devoted to Cu FeOz which was historically the first known compound exhibiting the so-called delafossite structure. Such a structure consists of close packed oxygen double layers in which the octahedral sites are occupied by Fe3+ cations. These double layers are linked by monovalent Cu+ ions with a two-fold oxygen linear coordination as shown in Fig. 1 (1, 2). * Permanent address: Applied Physics Department, Faculty of Sciences, King Mongkut Institute Technology, Lad-Kabang, Bangkok 10520, Thailand. 105
Magnetic properties have been intensively studied. CuFeOz is antiferromagnetic (TN = 13 K) with stronger interactions within the layers than along the c-axis, as could be anticipated from the structure (3). Calculations of the lattice energy and Messbauer spectroscopy measurements have confirmed the monovalent and trivalent oxidation states of copper and iron, respectively. The opto-electronic and electrical properties of p- and n-type polycrystalline Cu FeOz have been recently investigated, at room temperature, by Benko et al. (4). These authors have found that the carrier 0022-4596188
Copyright D 1988 hy Academic Prea, lnc All rights of reproductwn m any form reserved
FIG. 1. Delafossite-type cles represent the copper
mobility in p-type samples is much higher than that in n-type ones. They have attributed this behavior to two different conduction mechanisms involving Cu+ and Fe3+, respectively. Despite the 2D-character of the structure only one paper reports measurements of the anisotropy of transport properties of CuFeO? single crystals (5). Photoelectrochemical characterization and thermal variation of electrical properties of pure and Pt-doped single crystals reported here confirm the model of Benko et al. (4). Special attention is paid to the anisotropy and its variation with temperature. Sample Preparation
and Crystal Growth
CuFeOz polycrystalline samples have been prepared by solid state reaction between CuZO and Fez03 with the molar ratio 3: 1 as previously described (3). Pellets were sintered at T = 1325K for 48 hr in a silica tube sealed under vacuum and then quenched at room temperature. The Cu-delafossite-type compounds melt incongruently so that a flux method has been chosen for the single crystal growth. Examination of the Cu-Fe-O phase diagram shows the possibility of growing crystals from a copper rich flux of mixed oxides
in air (6). The starting oxides were CuO (Ultrapure from Alpha Ventron) and Fe103 (Specpure from Johnson Matthey). A mixture of thoroughly ground CuO and FezOj powder (wt. = 20 g) was introduced into a 30-cm’ platinum crucible and then heated in air. Starting composition, thermal cycle, and results are given in Table I. Only small size single crystals, referred to as Cx(Pt), could be obtained. They were separated from solidified copper oxide by leaching using hot diluted nitric acid for 7 days. The platinum crucible was attacked by the mixture and traces of Pt have been detected in the crystals as shown below. The main problems encountered using those experimental conditions result from (i) the high chemical reactivity of copper (I) oxide above 1300 K in the solid and particularly in the molten state (TM = 1398 K in air), (ii) the strong influence of the oxygen partial pressure on the CuZO/CuO equilibrium (7). The previous remarks led us to select a copper crucible and lithium metaborate as solvent. A mixture (wt. = 20 g) of LiBOz (Specpure), CulO (99.95% from Alpha Ventron), and Fez03 (Specpure from Johnson Matthey) was introduced into the crucible and heated in an alumina reaction tube swept by a flow (2 liters/hr) of dried argon (Po? = 10m4 atm). Growth conditions are summarized in Table I. Small single crystals, referred to as Cx(Cu), were easily recovered by washing with hot diluted nitric acid in an ultrasonic pot. In both cases the as-grown crystals were examined with an optical microscope in order to reject samples containing flux. The chemical composition of crystals from both growth methods has been confirmed by electronic microprobe analysis. As already mentioned traces of Pt were detected in Cx(Pt) single crystals. The Pt concentration is approximately of 0.08 mole’%
+ f Fe20q
0.04 01~0 + 0.04 + 0.92 LiBO,
Heating up to 1180°C at 5O”Cihr IO-hr soak at 1180°C Cooling down to 1020°C at 2”Cihr Final cooling down to room temperature at 3O”Cihr
Black hexagonal or triangular platelet5 with (001) principal faces and 2 x 2 x 0.3 mm’ size
Heating up to 950°C at 5O”Cihr IO-hr soak at 950°C Cooling down to 820°C at 2”C:hr Final cooling down to room temperature at 30”C/hr
Black platelets wjith (001) principal faces and 3 x 3 x 0.1 mm’ size
and homogeneously distributed in the crystal. The lattice parameters were determined on ground crystals from X-ray powder diffraction data with Si as standard. The parameter values, listed in Table II, are in a good agreement with a hexagonal cell of delafossite-type structure but show some small fluctuations which could be attributed to a slight departure from stoichiometry. The Ryrn space group has been confirmed on Weissenberg photographs. Experiments Electrical
The electrical conductivity measurements on polycrystalline samples have TABLE LATTICE
Ref. Polycryst. Cx(Pt) Cx(Cu)
II OF CuFeOz
4) 3.035 3.030 3.032
c(“b + 0.001
2 0.001 t 0.001
k 0.01 t 0.01
been carried out using the four-colinearprobe method and automatic equipment described elsewhere (8). In order to give evidence of the anisotropy of conductivity in single crystals which are plate-like shaped with the main faces perpendicular to the caxis, several methods have been used depending on the sample length in the current carrying direction. As the (TV conductivity measured in natural faces (i to c-axis) is isotropic, no problem arises from the contact position and the four collinear probe method is quite convenient. For conductivity measurements performed along the caxis (crl,)the contact position is more critical so that the Montgomery’s method apparently seems more appropriate (9). However, both methods were tried on Cx(Pt) single crystals which are relatively thick (~0.3 mm) and a quantitative agreement has been found between experimental results. For Cx(Cu) single crystals the thickness of which is about 0.1 mm the previous methods fail and the original pattern described by Rogers et al. appears to be more suitable (5). Nevertheless its application is restricted by the condition (rl 9 ~1
ciprocal temperature of polycrystalline samples and of the Cx(Cu) single crystals are compared in Fig. 2. For polycrystalline samples the conductivity follows an Arrhenius law in the 250500 K temperature range, the corresponding activation energy being AE = 0.41 eV. Between 500 and 750 K, d(log o)ld( l/T) first decreases and then increases for higher temperatures, suggesting a transition from an extrinsic to an intrinsic-type behavior. The electrical conductivity of Cx(Cu) single crystals has been measured from room temperature up to 850 K both parallely and perpendicularly to the c-axis (Fig. 2). The large anisotropy observed at T = 300 K (o,./ olI = 500) decreases at increasing temperature. The behavior of cri and (~11 vs lITgives evidence of temperature domains where the conductivities follow an Arrhenius law as observed before in the case of polycrystalline samples. Values of activation energy are given in Table III. The electrical conductivity of Cx(Pt) single crystals has been measured in the 7-800 K temperature range as shown in Fig. 3.
-1 -2-3-4 -5-6-
FIG. 2. Logarithm of electrical conductivity vs reciprocal temperature for CuFeOz single crystals [ref. Cx(Cu)]: (A) I to the c-axis, (W) 11to the c-axis, and for (0) polycrystalline samples.
which has to be satisfied as the equipotential planes are assumed to be parallel with the layers. If this condition is not fulfilled the two-probe method leads to more significant results. The variation of the conductivity vs reTABLE ELECTRICAL
Polycryst. (this work) Polycryst. 1% Sn (4) Cx(Cu) (this work) Cx(Pt) (this work) Polycryst. (4) Cryst. (5)
4.1 x 10-l -
n n P p -
9.4 2.8 8.9 9.3
x x x x
lo-‘(II) loo’ 10 ‘(III IO-T(1)
(1 assuming one type of carriers, h carrier number deduced from ( carrier number deduced from // parallel to c-axis. i perpendicular to C.-axis.
n (or p)” (cm ‘)
1.2 x lo”‘*
1.9 x 10-T
1.8 x lO”h
3.2 x IO-’
1.1 x 10-h
2.3 x IO ‘( ) 1.1 x IO-‘Y )
1.8 x ,o,y<
3.9 x lo”*
6.5 x 10~‘~~) 3.1 x 10 d(1) 25 (II) 96 (1) 1.53 3.3 x 10-q) 2 (1)
2.3x 5 x 10-l(1)
thermoelectric power Hall measurements;
I* V-l set
x IO fi
8.9 (II) 34 (I) 0.27 -
FIG. 3. Logarithm of conductivity vs reciprocal temperature for Pt-doped CuFeO? single crystals [ref. Cx(Pt)]: (A) I to the c-axis and (W) /I to the r-axis.
The anisotropy determined by Montgomery’s method is small (cr,/cr,, = 3.8 at T = 300 K) and nearly independent of temperature. Between 30 and 300 K the variation of log(c) vs 1000/T is linear. A departure from that behavior is observed near the Neel temperature (TN = 13 K) (3). The activation energy values below and above TN are given in Table 111. From 300 to 420 K the conductivities are nearly constant and slightly decrease for higher temperatures. Thermoelectric Power The thermoelectric power (Y of polycrystalline samples has been measured from 160 to 1000 K. As shown in Fig. 4, a! is negative in the investigated temperature range. The behavior of (Yvs 1000/T can be divided into two temperature ranges (170 < T < 6.50 and T > 730 K) corresponding to those observed for the conductivity variation. Inside those temperature domains Ia/ increases monotonically with reciprocal temperature. The activation energy of the thermoelectric power in the 160-300 K temperature range is much lower than that of the conductivity as shown in Table III. For Cx(Cu) single crystals the very small
thickness of the sample leads to a poor thermal contact between the sample and its holder when the thermal gradient is applied in the layer direction and consequently prevents one from making measurements in this direction. As a result, the thermoelectric power ~~11 could only be determined with the thermal gradient parallel to the c-axis. Between 190 and 300 K, (Y is negative and its absolute value decreases at increasing temperature (Fig. 4). The activation energy deduced from the thermoelectric power is higher than that of polycrystalline samples as shown in Table III. The thermoelectric power for Cx(Pt) single crystals could be measured from 10 to 300 K in both directions parallel and perpendicular to the c-axis. For T > 25 K the behavior of oil and (TV is similar: (Y is positive and increasing with temperature as shown in Fig. 5. Below 25 K, alI tends to zero while (Ye abruptly decreases becoming even negative at T = 25 K. Photoelectrochemical
The photoelectrochemical measurements were carried out in a 0.1 M Na2HP04 solu-
s b a "400-
-800 -1000 -
FIG. 4. Thermoelectric power ature for CuFeOz single crystals the c-axis and (0) polycrystalline
. .. . /u ** .:. 0.: .. .
vs reciprocal [ref. Cx(Cu)]: sample.
*._ .. *.
temper(D) I/ to
slightly higher than that determined by Benko and Koffyberg on a p-type CuFeO? polycrystalline sample (1.15 eV) (4). A more detailed study of the anisotropic behavior using polarized light with a face parallel to the c-axis as the surface electrode will be published elsewhere. -zoo-,
FIG. 5. Thermal variation of thermoelectric Pt-doped CuFeO? single crystals [ref. Cx(Pt)]: the c-axis. (U) (( to the c-axis.
i TMI power of (A) I to
tion (pH = 9.2) using an equipment described elsewhere (IO). A natural face perpendicular to the c-axis of a p-type single crystal Cx(Pt) was used as the active surface of the electrode. The quantity (nhv)“’ where 7 is the quantum efficiency is plotted vs photon energy hu in Fig. 6. The linear variation observed between 1.29 and 3.10 eV shows that the transition corresponding to the band gap is indirect with E, = 1.26 eV. This value is
3 ia ,’
FIG. 6. Determination of the energy single crystals [ref. Cx(Pt)].
The simplest hypothesis for explaining the p-type semiconducting behavior is to attribute the acceptor levels to the platinum atoms detected by electronic microprobe analysis. That hypothesis is supported by Hall effect measurements which lead to a carrier concentration equal to the Pt concentration. Using the classical equation c = nep
The electrical behavior of polycrystalline samples is relatively close to that of Cx(Cu) single crystals. In both cases the low electrical conductivity and negative thermoelectric power are thermally activated. On the contrary, Cx(Pt) single crystals have a positive thermoelectric power increasing with temperature and their electrical conductivity is very weakly activated.
gap for CuFeO:
one obtains the r.t. values of the mobility given in Table III. The difference in the mobility values (about one order of magnitude) between our results and those previously reported by Benko and Koffyberg, as shown in Table III, is not very surprising if we take into account (i) the difference in the nature of the samples: single crystals (this work) or polycrystalline samples (4), (ii) the difference in the doping elements and the sites they probably occupy: platinum in Cu+-planes (this work) or magnesium in Fe3+-planes (4), and
(iii) the determination methods of the number of carriers from Hall effect measurements in the present work and from thermoelectric power measurements in Ref. (4).
Fe or Cu :4s Fe :3d Donor level
The observed n-type semiconducting behavior of “pure” CuFeOz could be ascribed to oxygen vacancies leading to the formation of donor levels. The formation of Cu” is very unlikely since no other Cu-delafossite compound exhibits a n-type semiconducting behavior. Therefore, donor levels are rather Fe’+ ions more or less trapped in the vicinity of oxygen vacancies. For n-type semiconductors the thermoelectric power is given by
where No is the effective density of states in the conduction band, n is the carrier density, and the other quantities have their usual meaning. Assuming that the iron 3dband is sufficiently narrow so that the corresponding energy levels are degenerated, No has the same order of magnitude as the density of iron atoms, i.e., No = 2.2 x IO” cm ~j. The mobility values derived from Eqs. (I) and (2) are given in Table III. They are in agreement with that reported by Benko and Koffyberg for a n-type 1% Sn-doped sample (Table 111). Such low mobility values are characteristic of a hopping conduction mechanism. Therefore electrical transport near room temperature is likely due to electrons thermally excited into the Fe’. : 3d narrow band resulting from the tt,orbitals. This interpretation is in agreement with the very strong anisotropy observed in that temperature range: t$-orbitals are rather nonbonding and therefore a direct overlapping is only possible in planes per-
Cu :3d t-l FIG. 7. Schematic n-type CuFeO,.
pendicular to the c-axis. We shall see below that covalent bonding between 4s (iron) and 2p (oxygen) orbitals apparently decreases the anisotropy to a large extent. When temperature is raised. an intrinsic behavior seems to be reached (Fig. 2). However, the activation energy of the conductivity (A/Z” = 0.9 eV) is much higher than the value expected from photoelectrochemical measurements, i.e., E,/2 = 0.6 eV. Such a behavior can be understood only if we consider the electrical transport at high temperature to be governed by carriers excited into a conduction band of higher energy (.I??)where the mobility (p?) exceeds much of that of the lowest conduction band (p,). The corresponding energy diagram is schematized in Fig. 7. From r.t. measurements Benko and Koffyberg have proposed that the conduction band (corresponding to the band of energy El in Fig. 7) and the valence band result from the 3d-levels of iron and copper, respectively. Their interpretation is based on the difference of mobility values between nand p-type samples (4). The present results confirm such a mobility difference (Table III) which can be explained by the following considerations: -a very low mobility (p,) corresponding to a hopping-type transport is expected for the electrons occupying the 3d-orbitals
DORDOR ET AL.
of Fe3+ which have a rather localized character, -the much higher mobility (pV) of carriers in the copper 3d-levels (pV > 10s~, as quoted in Table III) can result from a relatively large overlapping of hybridized 3d,24s orbitals. ’ On the other hand the negative sign of thermoelectric power shows that the investigated temperature range p2 should be larger than p,. In such conditions the band at energy E2 could be identified simply with the 4s-band either of iron or copper. Then the strong covalent character of the Fe-O or Cu-0 bonds which are due to overlapping of the 4s-orbitals (more or less hybridized with 4p and 3d levels) with the 0: 2porbitals could explain why the anisotropy tends to disappear at high temperature.
Acknowledgments The authors are grateful to Dr. Lahaye for his contribution in EMA and to P. Keou for assistance in Hall effect measurements.
C. T. PREWITT,
ERS, Inorg. Chem. 10, 719 .I. P. DOKJMERC, A. AMMAR, POUCHARD,
I For a more detailed discussion see Ref. (5) where Rogers er al. show that the stabilization of the two-fold coordination of dl” cations is associated with a 3d,2-4s hybridization, the resulting orbitals having their electrostatic charge spread out in the copper plane. It may also be mentioned that Cu-Cu distances are close to the critical rc distance for localized vs delocalized states transition according to Goodenough (10) (neglecting the d,2-4s hybridization).
48, 37 (1987).
21, 745 (1986).
AND J. L. GILLSON, Inorg. Chem. D. S. BUST, A. M. M. GADALLA,
D. B. Roo-
J. P. DOUMERC, A. WICHAINCHAI, POUCHARD, AND P. HAGENMULLER,
4. F. A.
R. D. SHANNON,
C. T. PREWITT, 10, 723 (1971). AND J. WHITE.
35, 732 (1966).
R. D. SCHMIDT-WHITLEY, M. MENTE, AND A. REVCOLEVSCHI.
23, 113 (1974). 8.
P. DORDOR, E. MARQUESTAUT. P. HAGENMULLER, Rev. Phys.
(1985). 9. H. C. MONTGOMERY, J. Appl. Phys. (1971). IO. A. AMMAR, A. WICHAINCHAI, J. P. AND